Download presentation

1
**CHAPTER 3: CRYSTAL STRUCTURES & PROPERTIES**

Single Xtal Crystalline Poly-Xtal Materials Non-crystalline 1

3
**MATERIALS AND PACKING Crystalline materials...**

• atoms pack in periodic, 3D arrays • typical of: -metals -many ceramics -some polymers crystalline SiO2 Adapted from Fig. 3.18(a), Callister 6e. Noncrystalline materials... • atoms have no periodic packing • occurs for: -complex structures -rapid cooling "Amorphous" = Noncrystalline noncrystalline SiO2 Adapted from Fig. 3.18(b), Callister 6e. 3

4
**METALLIC CRYSTALS • tend to be densely packed.**

• have several reasons for dense packing: -Typically, only one element is present, so all atomic radii are the same. -Metallic bonding is not directional. -Nearest neighbor distances tend to be small in order to lower bond energy. • have the simplest crystal structures. We will look at three such structures... 4

7
**SIMPLE CUBIC STRUCTURE (SC)**

• Rare due to poor packing (only Po has this structure) • Close-packed directions are cube edges. • Coordination # = 6 (# nearest neighbors) (Courtesy P.M. Anderson) 5

8
**ATOMIC PACKING FACTOR • APF for a simple cubic structure = 0.52**

Adapted from Fig. 3.19, Callister 6e. 6

9
**BODY CENTERED CUBIC STRUCTURE (BCC)**

• Close packed directions are cube diagonals. --Note: All atoms are identical; the center atom is shaded differently only for ease of viewing. • Coordination # = 8 Adapted from Fig. 3.2, Callister 6e. (Courtesy P.M. Anderson) 7

10
**ATOMIC PACKING FACTOR: BCC**

• APF for a body-centered cubic structure = 0.68 Adapted from Fig. 3.2, Callister 6e. 8

11
**FACE CENTERED CUBIC STRUCTURE (FCC)**

• Close packed directions are face diagonals. --Note: All atoms are identical; the face-centered atoms are shaded differently only for ease of viewing. • Coordination # = 12 Adapted from Fig. 3.1(a), Callister 6e. (Courtesy P.M. Anderson) 9

12
**ATOMIC PACKING FACTOR: FCC**

• APF for a body-centered cubic structure = 0.74 Adapted from Fig. 3.1(a), Callister 6e. 10

13
**FCC STACKING SEQUENCE • ABCABC... Stacking Sequence • 2D Projection**

• FCC Unit Cell 11

14
**HEXAGONAL CLOSE-PACKED STRUCTURE (HCP)**

• ABAB... Stacking Sequence • 3D Projection • 2D Projection Adapted from Fig. 3.3, Callister 6e. • Coordination # = 12 • APF = 0.74 12

15
**STRUCTURE OF COMPOUNDS: NaCl**

• Compounds: Often have similar close-packed structures. • Structure of NaCl • Close-packed directions --along cube edges. (Courtesy P.M. Anderson) (Courtesy P.M. Anderson) 13

16
THEORETICAL DENSITY, r 14

17
Example: Copper Data from Table inside front cover of Callister (see next slide): • crystal structure = FCC: 4 atoms/unit cell • atomic weight = g/mol (1 amu = 1 g/mol) • atomic radius R = nm (1 nm = 10 cm) -7 14

18
**Characteristics of Selected Elements at 20C**

Adapted from Table, "Charac- teristics of Selected Elements", inside front cover, Callister 6e. 15

19
**DENSITIES OF MATERIAL CLASSES**

Why? Metals have... • close-packing (metallic bonding) • large atomic mass Ceramics have... • less dense packing (covalent bonding) • often lighter elements Polymers have... • poor packing (often amorphous) • lighter elements (C,H,O) Composites have... • intermediate values Data from Table B1, Callister 6e. 16

20
**CRYSTALS AS BUILDING BLOCKS**

• Some engineering applications require single crystals: --diamond single crystals for abrasives --turbine blades Fig. 8.30(c), Callister 6e. (Fig. 8.30(c) courtesy of Pratt and Whitney). (Courtesy Martin Deakins, GE Superabrasives, Worthington, OH. Used with permission.) • Crystal properties reveal features of atomic structure. --Ex: Certain crystal planes in quartz fracture more easily than others. (Courtesy P.M. Anderson) 17

22
POLYCRYSTALS • Most engineering materials are polycrystalline. 18

25
**Effect of grain size, an example**

26
**SINGLE VS POLYCRYSTALS**

• Single Crystals -Properties vary with direction: anisotropic. Data from Table 3.3, Callister 6e. (Source of data is R.W. Hertzberg, Deformation and Fracture Mechanics of Engineering Materials, 3rd ed., John Wiley and Sons, 1989.) -Example: the modulus of elasticity (E) in BCC iron: • Polycrystals 200 mm -Properties may/may not vary with direction. -If grains are randomly oriented: isotropic. (Epoly iron = 210 GPa) -If grains are textured, anisotropic. Adapted from Fig. 4.12(b), Callister 6e. (Fig. 4.12(b) is courtesy of L.C. Smith and C. Brady, the National Bureau of Standards, Washington, DC [now the National Institute of Standards and Technology, Gaithersburg, MD].) 19

29
Bar of Vanadium

30
Growing Crystals https://www.youtube.com/watch?v=l_USYub3djY

31
**Lattice Positions Example: cubic system**

32
**Procedure for finding direction:**

Select two points on the line End point - Start point Clear fraction Put in [hkl] format Note: negative sign goes above the number

33
**Example: Select two points on the line End point - Start point**

Clear fraction Put in [hkl] format

34
**Example: Select two points on the line End point - Start point**

Clear fraction Put in [hkl] format

36
**Procedure for finding planes:**

Find plane’s intercept with X, Y and Z axis Inverse the numbers Clear fraction Put in (hkl) format Note: negative sign goes above the number

37
**Find plane’s intercept with X, Y and Z axis**

Inverse the numbers Clear fraction Put in (hkl) format

38
**Find plane’s intercept with X, Y and Z axis**

Inverse the numbers Clear fraction Put in (hkl) format

40
**The previous equation of planar spacing is only for CUBIC systems.**

44
**Slip Direction (more later)**

Atomic Linear density, LD = (number of atoms/unit length) Slip Direction (more later) Calculate LD if cube is BCC

45
**Calculate LD if cube is FCC**

46
**Slip plane (more later)**

Atomic Planar density, PD = (number of atoms/unit area) Slip plane (more later) Calculate PD if cube is BCC

47
**Calculate PD if cube is FCC**

48
**Atomic Volume density, VD = (number of atoms/unit volume)**

Calculate VD if cube is BCC

49
**Atomic Volume density, VD = (number of atoms/unit volume)**

Calculate VD if cube is FCC

50
**Converting from/to cubic to hexagonal, Directions**

[hkl] and [uvtw] u=n/3(2h-k) v=n/3(2k-h) t=-(u+v) w=nl Example: covert [102] to hexagonal system U=n/3(2-0)=2n/3 V=n/3(0-1)=-n/3 t=-(2n/3-n/3)=-n/3 W=n(2) =2n

51
**Converting from/to cubic to hexagonal, plane**

(hkl) to/from (hkil) i=-(h+k) Example: convert (213) to hexagonal system

52
#atoms/UC a0 C.N P.F Elements SC 1 2R 6 0.52 BCC 2 8 0.68 Fe, W, Mo, Cr,… FCC 4 12 0.74 Fe, Cu, Al, Au, Ag, Pb, Ni,.. HCP a0 = 2R C0 = 3.266R Ti, Mg, Zn, Be, Co, Zr, ..

54
**X-RAYS TO CONFIRM CRYSTAL STRUCTURE**

• Incoming X-rays diffract from crystal planes. Adapted from Fig. 3.2W, Callister 6e. • Measurement of: Critical angles, qc, for X-rays provide atomic spacing, d. 20

56
**Watch this video: http://www. theguardian**

58
Graphical Methods

59
X-Ray: Another Method

60
Detection method n = 2dsin()

61
**Figure 3.22 Diffraction pattern for polycrystalline a-iron., a=0.29 nm**

n=2dsin() Example: Find wavelength of the x-ray used to generate the above graph.

62
**Pyrite (done with SEM at SSU)**

63
**SUMMARY • Atoms may assemble into crystalline or amorphous structures.**

• We can predict the density of a material, provided we know the atomic weight, atomic radius, and crystal geometry (e.g., FCC, BCC, HCP). • Material properties generally vary with single crystal orientation (i.e., they are anisotropic), but properties are generally non-directional (i.e., they are isotropic) in polycrystals with randomly oriented grains. 23

Similar presentations

Presentation is loading. Please wait....

OK

Chapter 3: The Structure of Crystalline Solids

Chapter 3: The Structure of Crystalline Solids

© 2018 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on series and parallel circuits video Ppt on ufo and aliens videos Ppt on interesting facts about maths Ppt on spiritual leadership training Marketing mix ppt on nokia cell Ppt on op amp circuits schematics Ppt on rfid based automatic car parking system Seminar ppt on paper battery Store window display ppt on tv Ppt on sugarcane industry